EFFECTIVE PERMITTIVITY TENSOR FOR A METAL-DIELECTRIC SUPERLATTICE

B. Zenteno-Mateo, V. Cerd´an-Ram´ırez and B. Flores-Desirena

Facultad de Ciencias F´ısico-Matem´aticas Benem´erita Universidad Aut´onoma de Puebla Apdo. Post. 1152, Puebla, Pue. 72000, Mexico M. P. Sampedro

Facultad de Ingenier´ıa Qu´ımica

Benem´erita Universidad Aut´onoma de Puebla C.U., Puebla, Pue. 72570, Mexico

E. Ju´arez-Ruiz

Facultad de Ciencias de la Electr´onica

Benem´erita Universidad Aut´onoma de Puebla C.U., Puebla, Pue. 72570, Mexico

F. P´erez-Rodr´ıguez

Instituto de F´ısica

Benem´erita Universidad Aut´onoma de Puebla Apdo. Post. J-48, Puebla, Pue. 72570, Mexico

Abstract—We have derived simple analytical expressions for the frequency-dependent effective permittivity tensor of a one-dimensional metal-dielectric photonic crystal in the long wavelength limit. Our results describe the transition between the regime, described by Rytov’s formulas for sufficiently long waves, and that predicted by Xu et al. [6], where the effective plasma frequency is independent of the metallic-layer parameters. The derived expressions can be useful for determining the frequency intervals where such an anisotropic system can exhibit metamaterial behavior.

1. INTRODUCTION

A very simple system for designing metamaterials is the periodic
heterostructure (also-known as superlattice or one-dimensional (1D)
photonic crystal (PC)) composed of alternating metal and dielectric
layers (see, e.g., [1–3]). In the regime of long wavelengths, compared
with the PC period*a, its optical properties can be described by using*
an effective permittivity tensor. If the permittivity components are
of different sign, such an anisotropic medium can support negative
refraction without requiring negative permeability [1–3], unlike
double-negative metamaterials. Commonly, the permittivity components are
calculated within the effective medium approach originally developed
by Rytov [4]. So, if the materials of the superlattice layers are local and
isotropic, the permittivity tensor is diagonal with principal values [4]:
*εx* = *εy* =*εmf*+*εd*(1*−f*), (1)

1
*εz* =

1*−f*
*ε _{d}* +

*f*

*εm.* (2)

Here, the metal and dielectric layers are characterized by their
permittivities, *εm* and *εd*, and thicknesses, *dm* and *d, respectively;*

*f* =*dm/a*is the metal filling fraction (a=*dm*+*d), andz* denotes the

direction perpendicular to the planes of the layers in the superlattice. Formulas (1) and (2) hold in the case of very long waves [4], and have also been obtained by using different homogenization methods (see, for example, [2, 5] and references therein).

Employing the Drude model for the frequency (ω)-dependent
dielectric function of the metal (i.e., *εm* = *ε*0(1*−ω _{P}*2

*/ω*2), where

*ωP*

is the metal plasma frequency, *ε*0 is the vacuum permittivity), the

components*εx* and *εy* (1) acquire a similar form:

*εx*=*εy* = ¯*εε*0

Ã
1*−* *ω*

2
*P,eff*

*ω*2

!

*,* (3)

with ¯*ε*=*f*+*εd*(1*−f*)/ε0 and an effective plasma frequency

*ωP,eff* =*ωP*

r
*f*

¯

*ε.* (4)

This result turns out to be good enough when the values of the filling
fraction are not very small (f *≤* 1). If *f* *¿* 1 and the metal layer
thickness is comparable with the skin depth (d*m* *∼c/ωP*), the cut-off

frequency*ω _{P}_{,}_{eff}* is close to the value [6]

where *n* = p*εd/ε*0 is the refraction index of the dielectric. Notice

that *ωP,eff* in Eq. (5) does not depend on the metal permittivity,

like the effective plasma frequency for periodic arrays of very thin
metal wires [7]. Although the differences between models (4) and (5)
have been analyzed in-depth [6, 8], up to now there are no simple
analytic expressions for the permittivity components, which can
predict both results as well as the crossover between them. In
principle, the two regimes could be described within the effective
medium approach proposed by Rytov [4]. However, the calculation
of the effective permittivity would require the numerical solution of
the exact dispersion equation, especially in the case of electromagnetic
modes propagating along the*z*axis [4] and having a low-frequency gap
in their photonic band structure.

In the present work, we will calculate the effective permittivity tensor for a binary metal-dielectric superlattice within the homoge-nization theory recently developed in the work [9]. This theory has the advantage of providing explicit expressions for the effective param-eters of the electromagnetic response. We shall apply it to study the plasma-like behavior of the metal-dielectric heterostructure.

2. THEORETICAL FORMALISM

According to the results, reported in [9], the effective *local*
electromagnetic response of a PC, which can be bianisotropic in the
most general case, is given by

¯¯
A*eff* =

" _{↔}

*ε _{eff}*

*↔ξ*

_{eff}*↔*

*ζ _{eff}*

*↔µ*

_{eff}#

*≡* lim

*k→*0

1
*ω*

n ¯¯

D*−*1(k; 0,0)
o_{−}_{1}

*.* (6)

Here, *↔ε _{eff}*,

*↔µ*,

_{eff}*↔ξ*, and

_{eff}*↔ζ*are, respectively, the effective permittivity, permeability, and crossed magneto-electric tensors, k is the wave vector, and

_{eff}*{. . .}−*1symbolizes the inverse of the 6

*×*6 matrix block ¯¯D

*−*1(k; 0,0), which is obtained from the inverse ¯¯D

*−*1(k;G,G

*0*

_{)}

of the infinite matrix ¯¯

D(k;G,G*0*) =

" _{↔}

0 (k+G)*×↔*I

*−*(k+G)*×↔*I *↔*0

#
*δ*_{G}_{,}_{G}*0*

+ωA(G¯¯ *−*G*0*), (7)
where G, G*0* _{are vectors of the reciprocal lattice of the PC,} _{δ}

G*,*G*0*

of the 6*×*6 matrix ¯¯A(r) for the material (bianisotropic) response:
¯¯

A(r)*≡*

" _{↔}

*ε* (r) *↔ξ* (r)

*↔*

*ζ* (r) *↔µ*(r)
#

*.* (8)

In the case of a binary metal-dielectric superlattice composed of
isotropic nonmagnetic materials, the crossed magneto-electric tensors
in Eq. (8) are 3*×*3 zero matrices, whereas the permeability tensor is

*↔*

*µ*=*µ*0
*↔*

I (µ0 is the vacuum permeability). Hence,

¯¯

A(G* _{z}−G0_{z}*) =
"

*εd*
*↔*

I *↔*0

*↔*

0 *µ*_{0} *↔*I
#

*δ _{G}_{z}_{,G}0*

*z*+ ∆ ¯¯A(G*z−G*
*0*

*z*), (9)

where

∆ ¯¯A(G* _{z}−G0_{z}*) =
"

∆ε*↔*I *↔*0

*↔*

0 *↔*0
#

*F*(G* _{z}−G0_{z}*), (10)
∆ε =

*εm*

*−εd*, and

*F*(G

*z*) =

*f*sin(G

*zdm/2)/(Gzdm/2) is the form*

factor of the metal layer.

The matrix block ¯¯D*−*1(0; 0,0) is obtained by numerically solving
the system of algebraic equations for the block column ¯¯D*−*1(0;*Gz,*0)

given by _{X}

*G0*
*z*

¯¯

D(0;*G _{z}, G0_{z}*) ¯¯D

*−*1(0;

*G0*0) = ¯¯Iδ

_{z},*(11)*

_{G}_{z}_{,0},where ¯¯I is the 6 *×*6 unit matrix. In order to physically interpret
our numerical results, we shall also derive a simple expression for the
effective permittivity tensor for the considered 1D PC, having thin
metallic layers. So, Eq. (11) can be rewritten as

*ω*T¯¯ *−*1(G*z*)

X

*G0*
*z*

∆ ¯¯A(G*z−G0z*) ¯¯D
*−*1

(0;*G0 _{z},*0) + ¯¯D

*−*1(0;

*Gz,*0)

= ¯¯T*−*1(0)δ* _{G}_{z}_{,0}.* (12)
Here, ¯¯T

*−*1(G

*z*) [10] is the inverse of

¯¯

T(G*z*)*≡*

"

*ωε _{b}*

*↔*I

*Gzz*ˆ

*×*

*↔*

I

*−Gzz*ˆ*×*
*↔*

I *ωµ*0
*↔*

I #

*.* (13)

Multiplying Eq. (12) by ∆ ¯¯A(*−Gz*) and summing over *Gz*, we get

*ω*X

*Gz*

∆ ¯¯A(*−Gz*) ¯¯T
*−*1

(G*z*)

X

*G0*
*z*

∆ ¯¯A(G*z−G0z*) ¯¯D
*−*1

(0;*G0 _{z},*0)

+X

*Gz*

It can be shown that in the case *f k _{d}a*

*¿*1 (i.e.,

*k*

_{d}d_{m}*¿*1), where

*k*=

_{d}*nω/c, the relation*

X

*Gz*

∆ ¯¯A(*−Gz*) ¯¯T
*−*1

(G*z*)∆ ¯¯A(G*z−G0z*)

*≈*

" * _{↔}*
S

*↔*0

*↔*

0 *↔*0
# "

∆ε*↔*I *↔*0

*↔*

0 *↔*0
#

*F*(*−G0 _{z}*), (15)

with (*↔*S)* _{ij}* =

*S*[S

_{i}δ_{ij}*=*

_{x}*S*= ∆ε d

_{y}

_{m}√µ_{0}

*/(2√ε*tan(k

_{d}

_{d}a)),*S*= ∆ε/(ωε

_{z}*)], is asymptotically correct. Using this relation in Eq. (14), we get*

_{d}X

*Gz*

∆ ¯¯A(*−G _{z}*) ¯¯D

*−*1(0;

*G*0) = "

_{z},¯¯ I+ω

"* _{↔}*
S

*↔*0

*↔*

0 *↔*0
##_{−}_{1}

∆ ¯¯A(0) ¯¯T*−*1(0). (16)

After substituting the sum (16) into (12) for *Gz* = 0, we obtain

an analytical expression for the matrix block ¯¯D*−*1(0; 0,0), whose
6*×*6 inverse matrix determines ¯¯A*eff* (Eq. (6)), having submatrices:

*εeff,ij* =*εiδij*,*µeff,ij* =*µ*0*δij*, and*ξeff,ij* =*ζeff,ij* = 0. The components

*εx* and *εy* of the effective permittivity can be expressed as

*εx* =*εy* =*εd*

1*−*

1
1*−* (ωa/2c)

*√*
*εd/ε*0
tanh(ωa/2c)*√εd/ε*0

i_{−}*εd*

*f*(ε*m−εd*)

*,* (17)

whereas our result for the component *εz* goes over into formula (2).

Besides, in deriving*εz* the condition*kddm* *¿*1 was not needed, unlike

the analytical calculation of *εx* =*εy* (17).

Notice that Rytov expression (1) for *ε _{x}* and

*ε*is obtained from Eq. (17) in the limit

_{y}*k*

_{d}a*→*0 as well as in the case of small metal filling fraction (f

*¿*1) and moderate dielectric contrast (i.e.,

*ε*

_{d}/f|εm*−*

*εd| À*1). However, as we will show below, at

sufficiently-large dielectric contrast, namely at *dm* *∼* *c/ωP* *¿* *d* (i.e.,

*ε _{d}/f|εm*

*−εd| ∼*(ω/ω

*P*)(ωd/c)

*¿*1), our formula (17) tends to the

permittivity (3) with the effective plasma frequency (5) proposed by Xu et al. [6].

3. DISCUSSION

0.00 0.05 0.10 0.15 0.20 0.25 -20

-15 -10 -5 0 5

ω/

P

x

/

0

3 2

1 3 2 1

ε

ε

ω

ω ω ω

Figure 1. Frequency dependence of the effective permittivity *εx* for

a metal-dielectric superlattice with *dm* = 0.5c/ω*P*, *d* = 10c/ω*P*, and

*n* = 1.5. The triangles and curve 1 were obtained by using Eqs. (6)
and (17), respectively. For calculating curve 2 [curve 3], we used the
model (3) with Eq. (4) [Eq. (5)]. *ω*1,*ω*2, and *ω*3 indicate the zeros of

*εx*(ω) corresponding to curves 1, 2, and 3.

a supperlattice with *dm* = 0.5c/ω*P*, *d* = 10c/ω*P* and *εd* = 2.25ε0

(n= 1.5) as that considered in [6]. Fig. 1 exhibits our numerical results
for the frequency dependence of the permittivity component*εx*(=*εy*)

[see triangles therein]. Evidently, the predictions of the formula (17)
(solid line, labeled with number 1 in Fig. 1) coincide with the numerical
results. Notice that *ε _{x}*(ω) has a zero at

*ω*=

*ω*

_{1}

*≈*0.121ω

*, which indicates the top or width of the low-frequency band gap (0*

_{P}*< ω < ω*

_{1}) in the photonic band structure for modes propagating along the growth direction of the metal-dielectric superlattice (Fig. 2). Interestingly, the dispersion relation

*k(ω) = (ω/c)*p

*εx/ε*0, calculated with the effective

permittivity (17), describes not only the low-frequency band gap,
but also the lowest pass band for photonic modes up to the middle
(ka/π *∼* 0.5) of the first Brillouin zone (see Fig. 2). We have also
calculated the effective permittivity*εx*(ω), given by Eq. (3), using the

cut-off frequencies (4) and (5) (see curves 2 and 3 in Fig. 1). As is
seen, the effective plasma frequencies*ω*2= 0.147ω*P* and*ω*3 = 0.209ω*P*,

predicted by such models, are larger than the exact result.

Figure 3 presents the dependencies of 1/ω*P,eff* (panel “a”) and

*ωP,eff* (panel “b”) upon the parameter*ωPnd/c, which were calculated*

0.0 0.2 0.4 0.6 0.8 1.0 0.0

0.1 0.2 0.3 0.4

ω

/

P

ka / 3

2 1

ω ω

ω

π ω

Figure 2. Solid line: photonic band structure for a metal-dielectric
superlattice as in Fig. 1. Dashed line: dispersion relation obtained by
using the effective permittivity*ε _{x}*(ω) (curve 1) from Fig. 1.

0 20 40 60 80 100

0 10 20 30 40

(a)

3

2 1

Pnd/c

P

/

P,eff

0 20 40 60 80 100

0.0 0.2 0.4 0.6 0.8 1.0

(b)

3

2

1

Pnd/c

/

P

ω ω

ω _{ω}

ω

ω

P,eff

Figure 3. Dependence of (a) 1/ω*P,eff* and (b)*ωP,eff* on the parameter

*ω _{P}nd/c*for a metal-dielectric superlattice with

*d*= 0.5c/ω

_{m}*. Curves 1, 2 and 3 were calculated by using Eqs. (17), (4), and (5), respectively.*

_{P}a homogeneous metallic medium with *ω _{P}_{,}_{eff}* =

*ω*if

_{P}*d→*0. On the other hand, at large values of

*ω*become parallel straight lines, and Rytov’s result considerably differs from our curve 1, which coincides with the reciprocal value of the cut-off frequency obtained from the exact photonic band structure. The slope of line 3 allowed Xu

_{P}nd/c, the curves 1 and 3 in Fig. 3(a)*et al.*to determine

*ωP,eff*(5) (see Fig. 2 in

[6]) with sufficiently accuracy. Indeed, the constant difference between
our result for 1/ω*P,eff* and the straight line 3 in Fig. 3, is negligible

the curves 1 and 3 in the panel “b” approach each other as *ω _{P}nd/c*
increases. The dotted vertical line in both panels of Fig. 3 indicates
the value of the parameter

*ω*= 15 which was used for calculating the graphs in Figs. 1 and 2 (and Fig. 1 in [6]). As is seen in Fig. 3(b), the value

_{P}nd/c*ωPnd/c*= 15 is in a relatively-broad interval where neither

formula (4) nor (5) predicts correct values for*ω _{P}_{,}_{eff}*.

In Figs. 4 and 5, we show the frequency-dependence of the effective
permittivity *εx* and the photonic dispersion for a superlattice with

the same parameters as in Fig. 1, except that *d* = 100c/ω*P*. Fig. 4

demonstrates the excellent agreement between analytical (curve 1)
and numerical (triangles) results. It is evident that in this case
the predictions by Xu et al. (Eqs. (3) and (5)) are very close to
our calculations of permittivity *εx*(ω) (compare curves 1 and 3 in

Fig. 4. In Fig. 5, one can observe that the effective plasma frequency
*ω*1 = 0.0193ω*P*, predicted by model (17), completely agrees with the

band structure calculations and is close to *ω*_{3} = 0.0209ω* _{P}* given by
Eq. (5). However,

*ω*

_{2}(4), obtained from Rytov’s formula (1), has a larger value (ω

_{2}= 0.047ω

*), being above the second pass band. The large difference between*

_{P}*ω*2 and the width of the low-frequency band

gap (see Fig. 5) is owing to the fact that in a metal with thickness*dm*

of the order of the skin depth (d*m* *∼c/ωP* *¿d) the condition of slight*

variation of the “microfield” across the metal layer, which was used in [4] in deriving formula (1), is not satisfied.

It should be commented that we have neglected damping effects,

0.00 0.01 0.02 0.03 0.04 0.05

-20 -15 -10 -5 0 5

/ _{P}

x

/

0

2 3

1

2 3

1

ω

ε

ε

ω

ω ω _{ω}

Figure 4. Frequency dependence of the effective permittivity *εx* for

a metal-dielectric superlattice with *dm* = 0.5c/ω*P*, *d*= 100c/ω*P*, and

*n* = 1.5. The triangles and curve 1 were obtained by using Eqs. (6)
and (17), respectively. For calculating curve 2 [curve 3], we used the
model (3) with Eq. (4) [Eq. (5)]. *ω*1,*ω*2, and *ω*3 indicate the zeros of

0.0 0.2 0.4 0.6 0.8 1.0 0.00

0.01 0.02 0.03 0.04 0.05

3 2

1

ka /

ω

/

P

ω

π ω

ω

ω

Figure 5. Solid line: Photonic band structure for a metal-dielectric
superlattice as in Fig. 4. Dashed line: Dispersion relation obtained by
using the effective permittivity*εx*(ω) [Eq. (17)].

which can be included in the Drude model by introducing a relaxation
frequency *ν, typically ranging in the THz region, as:* *εm* = *ε*0(1*−*

*ω _{P}*2

*/(ω*2+

*iων*)). Hence, the cut-off frequency will be well defined at frequencies

*ω*

*Àν, where losses in the metal inclusion are small. Drude*model is commonly used for bulk metal samples. However, this local model also describes the electromagnetic response of thin metal films (d

*m∼c/ωP*) in the optical range, since the effects of spatial dispersion

manifest themselves at much lower frequencies, namely in the THz region (see [11]).

4. CONCLUSION

In this work, we have applied the homogenization theory developed
in [9] to calculate the frequency-dependent effective*local* permittivity
tensor of a metal-dielectric superlattice. We could also derive analytic
expressions for the components of the permittivity tensor, describing
both the regime, where Rytov’s formulas [4] are valid, and that found
by Xu et al. [6] at very small metal filling fractions. Our results could
be useful in designing metamaterials based on metal-dielectric 1D PC.
ACKNOWLEDGMENT

REFERENCES

1. Podolskiy, V. A. and E. E. Narimanov, “Strongly anisotropic
waveguide as a nonmagnetic left-handed system,” *Phys. Rev. B,*
Vol. 71, 201101(R), 1–4, 2005.

2. Wood, B., J. B. Pendry, and D. P. Tsai, “Directed subwavelength
imaging using a layered metal-dielectric system,” *Phys. Rev. B,*
Vol. 74, 115116, 1–8, 2006.

3. Rakhmanov, A. L., V. A. Yampolskii, J. A. Fan, F. Capasso, and
F. Nori, “Layered superconductors as negative-refractive-index
metamaterials,”*Phys. Rev. B, Vol. 81, 075101, 1–6, 2010.*

4. Rytov, S. M., “Electromagnetic properties of a finely stratified
medium,”*Sov. Phys. JETP, Vol. 2, 466–475, 1956.*

5. Bergman, D. J. and D. Stroud, “Physical properties of
macroscopically inhomogeneous media,” *Solid State Phys.,*
Vol. 46, 147–269, 1992.

6. Xu, X., Y. Xi, D. Han, X. Liu, J. Zi, and Z. Zhu, “Effective
plasma frequency in one-dimensional metallic-dielectric photonic
crystals,”*Appl. Phys. Lett., Vol. 86, 091112, 1–3, 2005.*

7. Pendry, J. B., A. J. Holden, W. J. Stewart, and I. Youngs,
“Extremely low frequency plasmons in metallic mesostructures,”
*Phys. Rev. Lett., Vol. 76, 4773–4776, 1996.*

8. Manzanarez-Mart´ınez, J., “Analytic expression for the effective
plasma frequency in one-dimensional metallic-dielectric photonic
crystal,”*Progress In Electromagnetics Research M, Vol. 13, 189–*
202, 2010.

9. Cerd´an-Ram´ırez, V., B. Zenteno-Mateo, M. P. Sampedro,
M. A. Palomino-Ovando, B. Flores-Desirena, and F.
P´erez-Rodr´ıguez, “Anisotropy effects in homogenized magnetodielectric
photonic crystals,” *J. Appl. Phys., Vol. 106, 103520, 1–8, 2009.*
10. An explicit expression for ¯¯T*−*1(G) has been derived in Ref. [9]

(see Eqs. (33)–(37) therein).